1. API RP 571 (B)
51. ___________ are the most common type of equipment susceptible to carburization
in refining industry.
52. Different organisms thrive on different nutrients including inorganic substances
( Hydrocarbons, Organic acids). In addition, all organisms require a source of carbon,
nitrogen and __________ for growth.
53. In design and fabrication, it is advisable to avoid sharp changes in cross section,
such as short radius fillets or undercut that can give rise to _________. Long-seam
welds are particularly susceptible to reheat cracking due to mismatch caused by fit up
54. The most important factors affecting graphitization are the chemistry, stress,
temperature and _________.
Time at exposure
55. Creep damage is found in high temperature equipment operating above the
___________. Fired heater tubes and components, Catalytic reactors, FCC reactors
and FCC fractionator and regenerator internals all operate in or near this.
56. Amine stress corrosion cracking is most often associated with lean amine services.
The pure alkanolamine does not cause cracking. Cracking in rich amine services are
most often associated with _________ problems.
57. The loss in strength from spheroidization (Softening) is usually accompanied by
a(n) __________ in ductility, which allows for deformation at stress concentrations.
58. Which of the following materials is not susceptible to high temperature hydrogen
300 Series SS
59. Which of these materials are susceptible to creep damage?
Carbon Steel, Stainless steel, Low alloy steel
2. 60. High temperature hydrogen attack results from exposure to hydrogen at elevated
temperatures and pressures. The hydrogen reacts with __________ in steel to produce
__________, which cannot diffuse through the steel. The loss of carbides causes an
overall loss in strength.
61. Ferritic stainless steels are usually not used in ________ applications.
62. Stress ruptures are characterized by ___________ failures and are usually
accompanied by thinning at the fracture surface.
63. With hydrofluoric acid corrosion, corrosion rates increase with _________
temperature and ________ HF concentrations.
64. Which of the following materials is susceptible to CO
65. Steel hardness, __________ and stress are critical factors in causing hydrogen
66. If the BHN is 400-500 it may indicate__________.
67. The graphitization rate ________ with increasing temperature.
68. The level of creep damage is a function of the material and the coincident
_________ level at which the creep deformation occurs.
69. Titanium should not be used is known hydriding services such as ________ or
Amine, sour water
3. 70. Convert these temperatures - 156 degrees C and 450 degrees F
312 degrees F, 232 degrees C
71. Which of the following alkanoamine in causing amine corrosion?
72. __________ is a loss in toughness due to a metallurgical change that can occur in
alloys containing a ferrite phase, as a result of exposure in the temperature range 600
degrees F to 1000 degrees F.
885 degrees F embrittlement
73. Hydrochloric acid corrosion is a general and localized corrosion and is very
aggressive to most common materials of construction. Damage in refineries is often
associated with dew point corrosion in which vapors containing __________ and
hydrogen chloride condense from the overhead stream of distillation, fractionation, or
74. When connected to a more anodic material, titanium may suffer severe _________.
75. __________ is a form of stress corrosion cracking normally occurring during
shutdowns, startup or during operation when air and moisture are present. Cracking is
due to sulfur acids forming from sulfide scale, air and moisture acting on sensitized
Polythionic acid SCC
76. _________ usually occurs when a colder liquid contacts a warmer metal surface.
77. Which of these materials is not susceptible to amine cracking?
300 Series and 400 Series SS
78. The presence of ___________ in H2S streams increases the severity of high
temperature sulfide corrosion at temperature above about 500 degrees F.
4. 79. Increasing chromium content in the alloy improves resistance to sulfidation.
However, there is little improvement with increasing chromium content until about
80. ___________ is the sudden rapid fracture under stress (residual or applied) where
the material exhibits little or no evidence of ductility or plastic deformation.
81. Caustic embrittlement cracking can be effectively prevented by means of PWHT at
a temperature of __________.
1150 degrees F
82. General or localized corrosion of carbon steels and other metals caused by
dissolved salts, gasses, organic compounds or microbiological activity is called
Cooling water corrosion
83. With CO2 corrosion increasing temperatures __________ corrosion rates up to the
point where CO2 is vaporized.
84. Units where graphitization may be suspected are the FCCU and the ________ unit.
85. Where is PASCC normally located?
Adjacent to welds
86. All ________ based materials and low alloy materials, 300 Series SS and 400 Series
SS Re susceptible to Sulfidation.
87. Sulfuric acid promotes general and localized corrosion of carbon steel. Carbon
steel heat affected zones may experience severe corrosion. Acid concentration,
temperature, alloy content and __________ are critical factors affecting sulfuric acid
88. Which of these materials are susceptible to brittle fracture?
Carbon steels, Low Alloy steels, and 400 Series SS
5. 89. ________is a form of environmental cracking that can initiate on the surface of
high strength low alloy steels and carbon steels with highly localized zones of high
hardness in the weld metal and HAZ as a result of exposure to aqueous HF acid service.
Hydrogen stress cracking
90. HCI acid corrosion is found in several units, especially _________ and __________,
units, hydro-processing units and catalytic reformer units.
91. Cracking can occur at low caustic levels if a concentrating mechanism is present.
In such cases, caustic concentrations of ________ ppm are sufficient to cause cracking.
92. Which of these materials is susceptible to 885 degrees F embrittlement?
400 Series SS and Duplex SS
93. Spheroidization and graphitization are competing mechanisms that occur at
overlapping temperature ranges. Spheroidization tends to occur preferentially above
_________ while graphitization predominates below this temperature.
1025 degrees F
94. Sulfidation is primarily caused by ________ and other reactive sulfur species as a
result of the thermal decomposition of sulfur compounds at high temperatures.
95. Damage from sigma phase appears in the form of __________.
96. The extent and depth of decarburization is a function of temperature and
97. Corrosion of the anode may be significantly higher _________ to the connection to
the cathode, depending on solution conductivity.
98. Conditions favoring carburization include a high gaseous phase carbon activity and
_________ oxygen potential.
6. 99. Susceptibility to temper embrittlement is largely determined by the presence of
the alloying elements manganese and _________.
100. Improved resistance to erosion is usually achieved through increasing substrate
_______ using harder alloys, hard facing or face-hardening treatment.